High-Temperature Application of HENRY H. NELSON1
nitrocellulose lacquer has been the only deterrent to highsolids concentration, the breaking of that viscosity has eliminated the last obstacle. The resin accounts for only a small part of the lacquer viscosity, and resin solutions are reasonably thin a t high-solids concentrations. The use of nitrocellulose lacquer as a protective coating material is a result of the development of low viscosity nitrooottons, for the advent of ‘/Z-second nitromtton made the use of this fast-drying finish possible in the automotive industry. The high rate of motorcar production has been furthered by the rapid drying characteristic of nitrocotton lacquers. With the use of low-viscosity nitrocottons it became possible to spray lacquers a t from 12 to 18per cent solids. Previously it had not seemed possible to decrease the nitrocotton viscosities further so as to permit the spraying of higher solids. The reason is that the nitrocottons below ‘/4 second do not seem to have desirable durability properties. By the application of heat to reduce the viscosity of lacquers, it is now possible to spray from 28 to 40 per cent solids. This can be done, still retaining the working properties that make the use of nitrocellulose lacquers desirable.
Sharples Solvents Corporation, Philadelphia, Pa.
HE finishing of automobile bodies is a t present carried out by the following general procedure: (a) cleaning and preparation of the metal, (b) application of the primer followed by one or two coats of surfacer, and (c) a t least four coats of nitrocellulose lacquer enamel. The film thickness of the four lacquer coats may average about 1.5 mils or more. By means of the new technique of high-temperature lacquer application, it is possible to spray the equivalent of four normal coats of black enamel in one double application. A double application is considered as one vertical and one horizontal sweep of the spray gun over the work. The application of high-temperature lacquers to the finishing of motorcar bodies is an accomplished fact. Kot only has this method of applying high-solids lacquer been found experimentally possible on a laboratory scale, but the method is actually being tested on a production basis.2 The purpose of applying heat to lacquer is the reduction of the viscosity t o the point where relatively high concentration of solids can be applied to surfaces. As the viscosity of the
Principle of High-Temperature Lacquer The idea of high-temperature lacquer is soundly conceived. It is based on the sound principle that the viscosity of nitro-
Present address, Wyandotte, Mich. Bogin and Wampner, paper presented before 95th Meeting of American Chemical Society, Dallas, Texas, April 18 to 22, 1838. 1
cellulose solutions is sharply reduced a t somewhat elevated
2500 CHANGE OF VISCOSITY OF NITROCELLULOSE SOLUTIONS WITH TEMPERATURE.
CHANGE OF VISCOSITY OF NITROCELLULOSE S0LUTIO.NS WITH TEMPERATURE.
c.20-4 SOL N OF W E T ~ S E CNITROCELLULOSE I N AMYL ACETATE NORMAL*
A-rov, SOL N. OF SEC. NITROCELLULOSE IN AMYL ACETATE NORMAL.*
D=20% SOLN OF D R I E D ~ S E CNITROCELLULOSE IN AMYL ACETATE NORMAL
8-ZOOASOLN. OF WET 30-35 C P S . NITROCELLULOSE INAMYLACETATE NORMAL.*
?# A.S.1: M
*A S T M 0-318-36
FIQURE 1 70
temperatures. In order to establish the extent of the viscosity change and its behavior a t various temperatures, four nitrocotton solutions of various viscosities were prepared. Amyl acetate3 was used as a solvent, and all solutions were 20 per cent solids. Measurements were made by means of the Saybolt Universal viscometer. The results obtained are plotted on Figure 1. The break in viscosity is sharp until the area 40" to 50" C. is reached. At this point the drop tapers off somewhat but does not tend to level out sharply. Owing to the limitations of the equipment, no attempt was made t o determine the temperature a t which the viscosity of nitrocotton solutions becomes practically constant. Although such a determination might have some academic interest, it has no bearing on the immediate problem. The break in viscosity observed a t 70" to 80" C. is sufficient to justify the high-temperature application of nitrocellulose lacquers. Before passing judgment on the value of high-temperature lacquer application, the following list of objectives or requirements should be considered:
The panels used for the experimental work were of standard automotive body-gage sheet steel, 18 X 30 inches. These were thoroughly cleaned prior to the application of the first coat. The primer used was representative of the common metal body primers and was baked on. An oil base surfacer was used which required baking a t 180" F. (82' C.) for 20 minutes. The dry surfacer was water-rubbed with No. 320 wet or dry emery paper before the enamels were applied. To gain some preliminary information on the utility of high-temperature lacquer application, a standard type of black lacquer was used. The solids in this lacquer were kept constant while a wide variety of solvent formulations were tried. Preliminary trials using high-diluent type lacquers applied a t 28 per cent solids indicated definitely that nitrocellulose lacquers could be applied hot. As anticipated, the viscosity of the solutions was greatly lowered, and normally heavy-bodied lacquers could be sprayed a t higher temperatures with ease. The viscosity was broken sufficiently to permit free atomization a t the spray gun.
The finish must be equal in appearance to that obtainable with the typical lacquer systems now in use. The finish must dry sufficiently well t o be rubbed within the specified baking time (30 minutes at 180-225" F. or 82-107" (3.). I t must be possible t o rub the finish to a smooth glossy surface, free from excessive orange peel. Film thickness should be about 1.5 to 2.0 mils. The metallic tvnes ". should be free from "color float" and "mottling.!' The metallic lacquers must not show the objectlionable "scaling" or two-color ring formation when the surfacer is cut through wi3h a rubbing block. The desirable characteristics of lacquer surfaces must be retained. These are speed of drying, ease of rubbing, and ability to perform quick repairs. A fine surface orange peel is preferred to the large wave type, but the film must be well leveled out.
Formulas The initial work was done with standard lacquer-solvent combinations. Good panels were made by holding the spray gun fairly close to the work. Typical solvent formulations that gave satisfactory performance under ideal conditions were the following: Amyl acetate Amyl alcohol Toluene Amyl acetate $my1 alcohol Xylene Toluene
It has not been the purpose of this work to devise production-scale equipment for the use of high-temperature lacquers. The objective has been to demonstrate the feasibility of hightemperature application by means of laboratory panel work. The actual adaptation of the technique to the production line is rightly the task of the motorcar manufacturer in cooperation with his equipment suppliers.
Amyl aoetate Amyl alcohol Xylene Toluene
Butyl acetate Butyl alcohol Ethyl acetate Xylene Toluene
Toluene Butyl acetate Bmyl alcohol Butyl alcohol Amyl acetate
Application of Heat to Lacquer
in -_ 55 10 10
Amy acetate Methyl isobutyl ketone Amyl alcohol Toluene Amyl acetate Amyl aloohol Methyl isobutvl ketone Butyiacetate " Union Solvent No. 8 Xylene Amyl acetate Butyl acetate Amyl alcohol Toluene Union Solvent No. 8
10 5 65
10 10 10 40 20
% ;: 5 25 40
All of these formulas can be used in high-temperature lacquer formulation, and excellent panels can be made from these volatile combinations in any laboratory. The amount of solids employed throughout the work was usually about 28 per cent by weight. A typical blacklacquer of the following solids composition was used as a standard:
The method used in the laboratory for applying heat to the lacquer is simply to heat the material container in a hot water bath, The material container used was a quart capacity can on which pressure could be applied. The material was conducted from the pressure can to the gun by means of a Thiokol tube about 4 feet in length. The water bath was heated by bubbling live steam through the water for about 20 minutes in order to reach a temperature in the material container of from 80" to 90" C. At this temperature the material is ready for spraying. Application through the greater part of the experiments was a t pressures of 15 to 20 pounds on the material container and about 85 pounds a t the spray gun. The gun was a standard model with a nozzle designed to carry high-solids materials; otherwise every item was standard equipment and readily available from vendors.
l/esecond nitrocotton (dry basis) Ester gum Trioresyl phosphate
1 part 4 parts 10%
It is readily apparent to any formulator that this is not a durable automotive lacquer. I n addition, the high ratio of resin to nitrocotton is favorable to the making of high-solids lacquer solutions. Xevertheless, it was thought that in a preliminary examination of the volatile constituents the solids composition should be simple and standard throughout the series. This formula proved to be an excellent starting point for the work in hand.
a Specification8 for all amyl acetate in this report are A. 9. T. M. D318-30; for all amyl achohol, A. 5. T. M. D319-33.
INDUSTRIAL AND ENGINEERING CHEMISTRY
As was previously stated, these lacquers could be sprayed in such a manner as to obtain good results. When a gun technique was adapted that closely imitated conditions met with on the production line, it was found that “dusting” or overspray would be a major problem; that is, the dust from the overspray did not flow out well. It was apparent that a wet film was required and that an abundance of a slowly evaporating true solvent would probably be needed to minimize “dusting” and to redissolve the overspray that must inevitably be present. At this point it might appear to some that the volatile material could be made more wet by the addition of xylene. On the contrary, a slowly evaporating true solvent is required. A solvent is needed that will not only strike the work wet but will have the ability to redissolve and to “reflow” the partially dried particles of lacquer overspray. It is true also that a high-solids lacquer applied extremely wet will produce a high-gloss film with a deep, long, wavelike orange peel; but the technique of production spraying is such that the hot lacquer tends to be partly dry before it reaches the surface to be sprayed. With heated lacquers there is a high loss of volatile material between the gun nozzle and the work. Therefore, a wet lacquer has partially “set” when it hits the surface, and a highly volatile lacquer is dry. In fact, it sets so dryly that it becomes hard immediately and will not flow out further. This type of lacquer cannot be rubbed to a smooth surface. The wet lacquer will reflow particularly during baking, but it has set sufficiently to lack excessive flow. When the baking is started, it is necessary to have a high percentage of a high-boiling solvent present to reflow the ragged surface left as a result of the high air pressures used. This reflow will be especially effective if the remaining volatile material is a slowly evaporating, true solvent entirely free from residual diluent. The presence of a great deal of “trapped” heavy diluent at this point is likely to invite sagging; in any event, it contributes nothing to the flow. On the other hand, the presence of a considerable amount of a high-boiling solvent is a definite advantage. The presence of a true solvent keeps all the resin, nitrocotton, and plasticizer ingredients in a common solvent, permitting maximum leveling of a film free from structural imperfections. The gradual evaporation of the true solvent will keep the surface of the film open. Rapid loss of the solvent tends toward “skinning” or sealing over of the surface. When the trapped volatile material escapes, minute holes are formed which are referred to as pinholes. The presence of a slowly evaporating true solvent will prevent pinholing from developing in the film. Excessive flow from the use of large percentages of highboiling solvents, though anticipated, has not been encountered. The rate of evaporation between the gun and the surface is great. In fact, if no high-boiling solvent is present and the volatile constituent is composed largely of diluent or “low boiler,” the heated lacquer strikes the work hard and dry. AS the amount of “high boiler” is increased, the lacquer gradually becomes wetter and tends to level out better, I n fact, it is not impossible to spray a lacquer containing 100 per cent high-boiling solvent and no other volatile constituent except the alcohol originally in the wet nitrocotton. Such lacquers are not at all unreasonable, and the formulator, when designing lacquers for high-temperature application, might give some thought to that idea. The exact amount of high boiler to be used is directly related t o the problem of overspray. If overspray is excessive and proper flow is not obtained, the remedy is to increase the high-boiler content of the volatile material. On the basis of this experience, some improved solvent formulations for use in high-temperature lacquer application can be suggested:
Isopropyl aoetate Amyl acetate Xylene Union Solvent No. 8
36% 4 0 10 14
Ethyl acetate Amyl acetate sec-Butyl acetate Butyl aloohol Union Solvent No. 8
38% 20 25 5
Ethyl aoetate Amyl acetate Isobutyl acetate Isobutyl aloohol Union Solvent No. 8
VOL. 31, NO. 1 Isopropyl acetate Amyl aoetate Butyl aloohol Toluene
;E% 5 24
Amyl aoetate Ethyl acetate Amyl aloohol Toluene
Amyl acetate Isopropyl aoetate Butyl alcohol
Amyl acetate Amyl aloohol Ethyl soetate
Role of Diluents In view of the fact that the object of the entire program is to spray the maximum amount of solids, there seems to be but little justification for the presence of diluents which are primarily used to lower the material cost. They may be, and usually are, present as the vehicle for carrying the resins into solution. In very thin lacquer solutions their presence in high percentages does not add to the viscosity of the solution. However, when the spraying viscosity is high, the presence of diluents is somewhat detrimental in that the lowest viscosity in relation to the solids has not been obtained. Under the cold method of lacquer application, the true solvents played only a minor role in keeping the viscosity low. Because of the high ratio of volatile to solids, the viscosity was so low that the true solvent medium was present primarily to carry the nitrocellulose into solution. The sheer preponderance of volatile material kept the viscosity down within satisfactory spraying limits. Under these conditions a high amount of diluent could be used. The diluent did serve to keep the costs per gallon at a low figure. Since the diluents are not solvents for nitrocellulose, the logical pilan of attack, if maximum solids are wanted, is to eliminate all or most of the diluent. A great many formulas with varying percentages of diluent were tried. Considerable evidence was found t o support the use of 100 per cent true solvents in high-temperature lacquer formulation. I n fact, it is difficult to find a strong argument supporting the use of a diluent; the principal reason is probably convenience. The resins are normally dissolved and carried in stock in a coal-tar diluent. There seem to be no pressing reasons why this practice should be discontinued. This is particularly true if the final lacquer does not carry excessive amounts of diluent. It might also be noted that in high-solids lacquer technique there is no reason for adding additional diluent when the consumer adds thinner prior to spraying lacquer.
Composition of Volatile High-temperature lacquer technique, therefore, does permit a wide latitude of volatile formulation. Where a formulator is not restricted to one group of materials, it will be found essential for all-round good work to have at least 50 per cent of the volatile material as high-boiling true solvent. Under controlled conditions, somewhat less can be used. AS an example of the type of problem that is likely to be met, let us examine the following experiment: Lacquer A (a standard automotive lacquer) was made up with the following volatile composition: Diluent
Low- and medium-boiling solvent
To this lacquer, 25 per cent by volume of the following thinner was added:
INDUSTRIAL AND ENGINEERING CHEMISTRY
After heating and spraying, this lacquer gave a film that had a dry and dusty surface. It was impossible to “wheel” this down to an acceptable finish in spite of the fact that i t contained almost 30 per cent of a high-boiling solvent. This result was obtained by holding the gun well back from the work so as to duplicate the overspray conditions encountered on the production lines. It might be well to emphasize that it would have been possible to make a passable panel by holding the spray gun close to the work. In spite of this, every effort was made to duplicate the technique characteristic of production work and to base the observations on the results obtained. A second trial was conducted with the same black lacquer enamel. Again the reduction was 25 per cent by volume. The reducer was composed of 70 per cent amyl acetate and 30 per cent diluent. This panel, with the gun held back from the work, received an excellent finish. Atomization a t the gun was good and the material was sufficiently wet to permit flexibility in the gun technique, The lacquer required no “babying” on the part of the operator. The colored lacquers experimented with, gave no trouble not readily solved on the basis of the experience gained during the experiments with black lacquers. A great many tests with a group of standard automotive lacquers were performed with amyl acetate and other solvents as the thinners. This method of attack was used to gain quickly preliminary information that might be encountered in hot lacquer application. On the basis of this work, a generalization can be safely made: The higher the amyl acetate ratio in the entire volatile, the more satisfactory the final film will be. This was carefully determined after carrying out the same spraying technique that was developed under the subject of black lacquers. I n fact, with amyl acetate as the sole thinner it was possible to obtain freedom from orange peel that was unusual. The rubbing required was in many cases reduced to a minimum. It is not necessary to reformulate most standard lacquers for high-temperature application, but it would seem that some effort should be made to put most of the highboiling solvents required into the basic lacquer. It may prove difficult to sell a lacquer to the consumer which requires that he purchase a high-price solvent, The automotive industry is so accustomed to cut-rate thinners that a mental resistance to the new prices might be built up in the buyer’s mind, although in spite of the higher cost per gallon there would still be a saving due to the lower total volume of thinner used. At any rate, it would seem logical for a lacquer producer to supply lacquers for high-temperature work containing the maximum practical amount of high-boiling solvent. In no other way can the manufacturer be assured that his lacquers will always give reasonably good effects, even though some off-grade thinners are occasionally used with his products. To obtain a preliminary observation on the limits, if any, of high-boiling solvent that can be used in the base lacquer, the following test was carried out: A typical lacquer was formulated with amyl acetate as the sole solvent. The resins were cut in amyl acetate as well as the nitrocotton. The entire lacquer was then reduced to about 38 per cent solids, using amyl acetate as the thinner. Heat was applied to the lacquer, and a panel, 18 X 30 inches, was sprayed. This panel had previously been prepared with a primer and a baking sudacer properly sanded. It was possible to apply a heavy, full film of lacquer with no evidence of sagging or of the large wavy type of orange peel. Furthermore, there was no indication of lifting of the undercoat by the lacquer. It was entirely reasonable to expect that the high concentration of amyl acetate in the film might possibly cause lifting of the oil base surfacers. I n no case, regardless of the solvent con-
centration, was lifting encountered during the spraying of over two hundred panels with high-temperature lacquer, It is apparent from these observations that there is no upper limit to the use of a high-boiling solvent, such as amyl acetate. The formulator can employ all of the amyl acetate that his cost schedule and manufacturing technique will permit. Perhaps the minimum of amyl acetate in the base lacquer should be placed a t about 50 per cent of the volatile portion. This will ensure a reasonably good performance on the job in the event that some inferior thinners are used by the consumer. A typical lacquer volatile which might be suggested is as follows: Amyl acetate sec-Butvl acetate
20 20 5
Metallic Lacquers When the work on high-temperature lacquer application was being planned, it was thought that the two extremes would be represented by the black lacquers and the metallic types. All the plain colors could be handled on the same basis as the black lacquer enamel. It was rightly felt that the metallic finishes would offer considerable difficulty. Under the present method of low-solids application, special care must be exercised in the spraying of metallics to prevent scaling or ring formation. The phenomenon known as scaling is a two-color effect which develops if the film is cut through during the rubbing. This condition is encountered where excessive floating of the aluminum particles has occurred, leaving a light layer of aluminum near the surface with a deep layer just below. I n production, the spots that are inadvertently cut through by the rubbing block must be touched up again. If excessive floating occurs in the metallic lacquer, the touch-up spots cannot be rubbed out properly, A two-tone effect will then be visible, and the paint job on that motorcar will be rejected by the inspectors. This is not a new situation and has been a constant source of annoyance sinoe the first use of metallic finishes on motorcars. The work done a t this laboratory on a great variety of commercial metallic finishes showed definitely that gun technique is still of primary importance in spraying this class of finishes. In fact, it may not be possible to produce satisfactory metallic finishes with one double application. It may be necessary to spray one wet coat followed by several dry applications of the metallic lacquer. This work has shown that it is necessary to use a high-boiling solvent that will permit wet spraying, just as was the case with black and colored lacquers. The technique followed was to apply a full wet coat, then finish by spraying dry into the wet hackgronnd. The operation can readily be accomplished by holding the gun close to the work initially and drawing the gun away for the final applications. That technique eliminates floating by causing the top layers of lacquer to be partially set. The presence of the residual high-boiling solvent adequately handles the overspray, as was demonstrated during t,he black lacquer work. The use of high ratios of a good high-boiling solvent permits greater flexibility of the gun manipulation. If the lacquer has a rather large amount of a low-boiling solvent, great care must be used or a dry, pebbly surface will he obtained that cannot be properly rubbed out. The high-boiling solvent present is an assurance that the film will level out and that the dry spray will be redissolved so as to permit satisfactory rubbing of the surface. Through the use of amyl acetate, the lacquer can be set partially so as to prevent flotation of the aluminum particles to the surface. Because of the strong solvent power and the slower evaporation rate of amyl acetate, the fdm can be reflowed. This process is especially con-
INDUSTRIAL AND ENGINEERING CHEMISTRY
ducive to good leveling when the finish is dried by heat in the baking oven. Some authorities with whom this subject was discussed contended that high-boiling solvents in metallic finishes would not prove feasible. Their theory was based on the likelihood that a high-boiling solvent would keep the film so wet that the aluminum particles would float to the top and invariably give the two-color condition. Had this contention proved correct, the application of metallic lacquers by the use of high temperatures would have been impossible. It is true that an improper and excessively wet application will cause color floating of metallic lacquers so that gun technique again must be relied upon for the best results. The extensive work done a t this laboratory has conclusively shown that with the proper gun technique the liberal use of amyl acetate permits more flexibility of action to the spray gun operator. A dry solvent is dangerous, for poor work is sure to result unless extreme care is exercised. A slowly evaporating solvent permits the use of a technique that is consistent with present practice, and good flow will always be assured. The spray operator will not be required to learn a new technique if a sufficiently wet lacquer is used, but the lacquer must be wet with true solvents and not slowly evaporating diluents. It is, however, possible t o use moderate percentages of slow diluents in the presence of a solvent similar to amyl acetate. A few examples of panels selected a t random from the work with the metallic type lacquers will illustrate the results obtained : PANEL 83. Metallic brown, manufactured by B. Reduced in the ratio 4 parts of enamel to 3 of the following thinner: Isobutyl acetate Isobutyl alcohol Toluene Union Solvent No. 8
35% 35 15 15
This material was difficult to spray, and showed the pinholing effect and scaling. PANEL84. Metallic brown, manufactured by B. Reduced in the ratio 4 parts of enamel to 3 of thinner: Amyl acetate Isobutyl acetate Union Solvent No. 8
25% 50 25
This was a satisfactory panel in every way. PANEL 87. Metallic blue, manufactured by A. Reduced in the ratio of 4 parts of enamel to 3 of thinner: Amyl acetate Toluene
This wa8 a satisfactory panel. PAKEL88. Metallic brown, manufactured by A. Reduced in the ratio of 4 parts of enamel to 3 of thinner. Amyl acetate, 100 per cent. This was an excellent panel without a single indication of scaling. Dispersion at the gun was perfect. PANEL133. Gun-metal metallic, manufactured by B. Reduced in the ratio of 4 parts of enamel to 3 of thinner: Amyl aoetate E t h y l acetate Union Solvent No. 8
$% ; 30
This was a satisfactory panel. PANEL140. Gun-metal metallic, manufactured by B. Reduced in the ratio of 4 parts of enamel t o 3 of thinner: Amyl acetate E t h y l acetate
2 parts 1
This panel had excellent leveling and was free from scaling. PANEL 141. Gun-metal metallic, manufactured by B. Reduced in the ratio of 4 parts of enamel to 3 of thinner: Butyl acetate Ethyl acetate
2 parts 1
This was rough and free from scaling, and had an orange peel which was difficult t o rub out. PANEL149. Gun-metal metallic, manufacturer B. Reduced in the ratio of 4 parts of enamel to 3 of thinner: Isobutyl propionate Amyl acetate
This was an excellent rubbing surface and was free from scaling.
VOL. 31, NO. 1
PANEL 152. Green metallic, manufacturer C. Reduced in the ratio of 4 parts of enamel to 2 of amyl acetate. This was an excellent panel in every respect.
Reductions and Viscosity U p to this point the question of reductions and viscosity for spraying has been avoided for the sake of simplicity. Present; spraying practice is almost universally based on reducing t h e lacquers to viscosities of 18 to 22 seconds on the No. 4 Ford. cup. Many technicians insist that 18 seconds is the maxi-. mum viscosity that should be used for best atomization at. the gun. During the initial stages of the high-temperature lacquer work, viscosity measurements were ignored. The crux of the. problem was to get the maximum amount of solids on the, surface being coated. No previous experience with highsolids lacquer existed. Therefore, if lacquers could be made. to spray a t nearly 30 per cent solids, other attendant details. for control could be worked out later. Nearly all the preliminary work was done by reducing the lacquers in the ratio.? of 4 parts of enamel to 3 parts of thinner. Considerable work has been carried out on this basis with good results. Since experience had been gained through the success of thepreliminary work, the use of rich thinners and reductions aslow as 4 to 2 and 4 to 1.5 were tried. These reductions, particularly with amyl acetate, proved to be very satisfactory. At this point it was thought that the maximum solids had been reached and that some practical method for control of" the high-temperature spraying should be adopted. There-. fore, viscosity readings on the KO.4 Ford cup were correlated. with the practical spraying results obtained. Viscosity readings were taken on the reduced lacquers a t room tempera-. tures in all cases. It would be difficult to obtain viscosityreadings on the hot lacquer, and the results would be of n o practical value; that is, although such information is of academic interest, i t could not be used as a means of control in the paint room. Viscosity readings at room temperature. can easily be taken, and they permit some control over the. thinning operation. If a reading of 60 seconds has been found satisfactory for spraying a specific lacquer, thinners can readily be added until this viscosity is reached. There may be times when several readings will be required before the proper amount of thinner has been added. This is the general tech-. nique for control employed at present, and once a viscosity. has been correlated with workability, there should be no fur-. ther difficulty. After spraying a great many test panels from a wide variety of lacquer enamels, it was concluded that viscosities around 70 seconds represented the maximum practical viscosity.. With some lacquers, using amyl acetate as the only thinner, success was had in the 70-second range, but for most work viscosities running from 60 t o 65 seconds give good results. This does not exclude the use of viscosities below 60 seconds. Some excellent results were obtained in the 50-60 second range, The following lacquers on which viscosity readings, were made will illustrate these conclusions: PANEL 155. Gun-metal metallic, manufacturer B. The lac-. quer reduced in the ratio of 4 to 2 with isobutyl propionate. Viscosity obtained in the No. 4 Ford cup was 67 seconds. The material did not atomize as freely as it should, but the final film would be rated fair. PAKEL156. Gun-metal metallic, manufacturer B. Reduced 4 t o 2 with amyl acetate. Viscosity with the No. 4 Ford cup. was 55 seconds. There was excellent atomization at the gun and good leveling on the panel surface. PANEL 159. Gray metallic, manufactuer D. Reduced 12 to' 4, or 331/a per cent by volume, with butyl acetate. Viscosity. with the No. 4 Ford cup was 61 seconds. The spraying was unsatisfactory. There was bad flooding of the color, and the" dried panel showed excessive pinholing and practically no flow.. This panel could not be accepted as being of any value.
INDUSTRIAL AND ENGINEERING CHEMISTRY
PANEL 160. Gray metallic, manufacturer D. Reduced 4 to 37.5 per cent by volume, with amyl acetate. Viscosity with the No. 4 Ford cup was 67 seconds. The spraying property was excellent. Flow and leveling were good. After a light rub, this panel presented a good appearance and did not show ring formation or scaling on the spot rubbed through. 11/2,
Amyl acetate appears to have a marked effect on dispersion a t the gun nozzle. It cannot be demonstrated on paper, but the operator observed this phenomenon. The finished panels also show the results of better atomization when amyl acetate is present in the lacquer. Butyl acetate a t a viscosity of 61 seconds with the No. 4 Ford cup failed to disperse properly and produced a poor film. Amyl acetate a t 67 seconds viscosity with the same cup produced a panel that required little rubbing. Isobutyl propionate a,t 67 seconds with the No. 4 Ford cup produced a panel that was satisfactory, but it seemed a little heavy a t -that viscosity for general use. Apparently, the slower evaporation rate of the amyl acetate serves the purpose of keeping the film open sufficiently long t o permit escape of the volatile constituent. The presence of a true solvent a t the end permits a general reflow of the film and keeps the film surface from sealing over: PANEL165. Black lacquer enamel, manufacturer -4. Reduced 4 t o 1 with a thinner consisting of 70 per cent amyl acetate and 30 per cent LTnion Solvent No. 8. The viscosity with the No. 4 Ford cup was 65 seconds. The results were good, but it seemed rather heavy for the best spraying efficiency, The panel leveled out and roved to be satisfactory. PANEL 166. hack lacquer enamel, manufacturer D. Reduced 4 t o 1 with: Toluene Ethyl alcohol Methyl ethyl ketone Butyl alcohol Amyl acetate
% ;: 25
Viscosity with the No. 4 Ford cup was 52 seconds. I t was sprayed dry with a fine orange peel. The surface was so hard and rough that it was difficult to cut down with the rubbing block. This material proved entirely too dry for production use. PANEL167. Gray metallic, manufacturer A . Reduced in the ratio 16 to 5 with amyl acetate. Viscosity with the No. 4 Ford cup was 82. This was too heavy for satisfactory spray application. PANEL168. Same material as used in panel 167. Reduction was 16 to 6 with amyl acetate. Viscosity with the No. 4 Ford CUD was 67 seconds. This reduction resulted in an excellent panel inevery way. Little rubbing was required t o bring up a good surface. PANEL 169. Gray metallic, manufacturer A . Reduction was 16 to 5 with:
Viscosity with the KO. 4 Ford cup was 67 seconds. This was entirely too dry for satisfactory use. PANEL170. Tan polishing lacquer, manufacturer A . Reduced 15 to 6 with a thinner consisting of 75 per cent amyl acetate and 25 per cent methyl ethyl ketone. Viscosity with the No. 4 Ford cup was 64 seconds. This panel turned out well. but the use of 100 per cent amyl acetate would have given better atomization at the gun nozzle. PANEL171. Tan polishing lacquer, manufacturer A . Reduced 15 t o 7 with amyl acetate. Viscosity with the No. 4 Ford cup was 72 seconds. This was a satisfactory panel. In spite of the relatively high viscosity, atomization was adequate for a good panel to be made. Because of the variation among competitive lacquers and the slightly different conditions under which each is used, it has not been considered advisable to make exact formula recommendations. The purpose of the work has been to establish the practicability of high-temperature application. Parallel with this objective, some general principles have been established that may govern the use of solvents.
Throughout this work the old idea of formulating for solvent balance has been abandoned. It has been definitely established that the evaporation of volatile material from a film is initially rapid and that the end is greatly delayed. This is true regardless of the solvent or solvent blend used. Flow and leveling of a film are not functions of solvent balance. Flow is due primarily t o the nature of the residual volatile constituent remaining in the film at the end of the drying period. It has been demonstrated that good performance in hightemperature lacquer work is based largely on the presence of high-boiling solvents. The lower limit for satisfactory performance has been established a t about 50 per cent of the total volatile material. The upper limit is where the individual formulator feels he has achieved a sufficiently wet condition. It has been shown also that 100 per cent high boiler can be used with excellent success in all high-temperature lacquer work. Amyl acetate is an ideal solvent for hot lacquer application in automobile finishing systems. This is due to its low vapor pressure and its even raLe of evaporation from the film. The use of amyl acetate mill ensure a wet film when the lacquer strikes the surface being coated. This is important, as the lighter and more volatile solvents vaporize from the hot atomized spray very quickly, and it is probable that the low-boiling solvents are evaporated before they strike the surface. Unless an adequate percentage of a relatively slow-evaporating solvent is present, a dry film with a dusty or sandy surface is likely to result. A ragged dry film cannot be rubbed and polished to a smooth surface. The presence of from 20 to 50 per cent of amyl acetate in the volatile portion of any lacquer formulation will increase its flow and leveling properties. This is a general statement and has been substantiated during the spraying of about two hundred and fifty panels with lacquers of as many different volatile combinations. It is not absolutely essential to reformulate the present lacquers for high-temperature lacquer applications. Present enamels may be used by thinning with thinners rich in high-boiling solvents. A great many lacquers have been purchased on the market and used with thinners containing as high as 70 per cent amyl acetate and the balance diluent. A formulation that has been successful and is cheap consists of 25 per cent amyl acetate, 50 per cent sec-butyl acetate, and 25 per cent diluent. Experimental work with a gun-metal metallic lacquer, specifically designed for high-temperature work, clearly demonstrated that amyl acetate is of particular value for this purpose. The results may be summarized as follows : Amyl acetate is valuable for the development of smooth films requiring a minimum of rubbing for good results. Amyl acetate does not cause the two-color effect frequently observed when the lacquer film is rubbed through under the high speed buffer. Amyl acetate definitely aids the proper atomization of the high-solids lacquers a t the spray gun nozzle, and is of vaIue to redissolve and reflow the “dusty” first coat or overspray. There is evidence to show that amyl acetate invariably aids in breaking up metallic lacquers so as to obtain a uniform distribution of the aluminum particles throughout the film. The use of 100 per cent amyl acetate will aid in the production of lacquer films free from the two-color effect. This is true when the proper gun technique is employed.
Acknowledgment Acknowledgment is made to John Marshall, E. I. du Pont de Nemours & Company, Inc., for advice and aid in the preparation of this paper. RECEIVED October 24, 1938